#------------------------------------------------------------------------------
#$Date: 2021-09-06 14:13:55 +0300 (Mon, 06 Sep 2021) $
#$Revision: 268770 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/70/74/7707474.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7707474
loop_
_publ_author_name
'Li, Jia-Nian'
'Du, Ze-Yu'
'Li, Ning-Fang'
'Han, Ye-Min'
'Zang, Ting-Ting'
'Yang, Mu-Xiu'
'Liu, Xiao-Mei'
'Wang, Ji-Lei'
'Mei, Hua'
'Xu, Yan'
_publ_section_title
;
 Two three-dimensional polyanionic clusters
 [M(P₄Mo₆)₂] (M = Co, Zn) exhibiting
 excellent photocatalytic CO₂ reduction performance.
;
_journal_issue                   26
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9137
_journal_page_last               9143
_journal_paper_doi               10.1039/d1dt00809a
_journal_volume                  50
_journal_year                    2021
_chemical_formula_sum            'C30 H71.33 Co5.33 Mo12 N12 O70 P8'
_chemical_formula_weight         3433.65
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2021-05-13 deposited with the CCDC.	2021-05-24 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 123.811(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   30.375(4)
_cell_length_b                   14.5133(14)
_cell_length_c                   24.714(3)
_cell_measurement_reflns_used    7746
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      53.651
_cell_measurement_theta_min      4.369
_cell_volume                     9052.4(19)
_computing_cell_refinement       'SAINT (Bruker, 2005)'
_computing_data_collection       'APEX2 (Bruker, 2005)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    SHELXTL
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2018/3 (Sheldrick, 2018)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker Apex2 CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0620
_diffrn_reflns_av_unetI/netI     0.0462
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       36
_diffrn_reflns_limit_h_min       -36
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            32307
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.614
_exptl_absorpt_coefficient_mu    2.809
_exptl_absorpt_correction_T_max  0.771
_exptl_absorpt_correction_T_min  0.683
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 2003)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    2.519
_exptl_crystal_description       blocky
_exptl_crystal_F_000             6653
_exptl_crystal_size_max          0.150
_exptl_crystal_size_mid          0.120
_exptl_crystal_size_min          0.100
_refine_diff_density_max         2.307
_refine_diff_density_min         -1.808
_refine_diff_density_rms         0.268
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.094
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     648
_refine_ls_number_reflns         8040
_refine_ls_number_restraints     311
_refine_ls_restrained_S_all      1.395
_refine_ls_R_factor_all          0.0714
_refine_ls_R_factor_gt           0.0575
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1008P)²+130.8909P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1630
_refine_ls_wR_factor_ref         0.1742
_reflns_Friedel_coverage         0.000
_reflns_number_gt                6542
_reflns_number_total             8040
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d1dt00809a2.cif
_cod_data_source_block           JW-20
_cod_depositor_comments
'Adding full bibliography for 7707474--7707475.cif.'
_cod_original_cell_volume        9052.5(17)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               7707474
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.678
_shelx_estimated_absorpt_t_max   0.766
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.13308(3) 0.61300(5) 0.47609(3) 0.0209(2) Uani 1 1 d . . . . .
Mo2 Mo 0.19140(3) 0.96110(5) 0.39245(4) 0.0238(2) Uani 1 1 d . . . . .
Mo3 Mo 0.14038(3) 0.76884(5) 0.53134(4) 0.0235(2) Uani 1 1 d . . . . .
Mo4 Mo 0.17718(3) 0.96990(5) 0.48648(4) 0.0253(2) Uani 1 1 d . . . . .
Mo5 Mo 0.17810(3) 0.75378(6) 0.31406(3) 0.0237(2) Uani 1 1 d . . . . .
Mo6 Mo 0.15261(3) 0.60666(6) 0.34974(4) 0.0309(2) Uani 1 1 d . . . . .
Co1 Co 0.250000 0.750000 0.500000 0.0190(3) Uani 1 2 d S . P . .
Co2 Co 0.000000 0.92498(13) 0.250000 0.0369(5) Uani 1 2 d S T P B .
Co3 Co 0.03440(7) 0.76330(14) 0.21079(10) 0.0353(5) Uani 0.6667 1 d . U P B .
Co4 Co -0.03982(5) 1.02610(9) 0.40815(6) 0.0280(3) Uani 1 1 d . . . . .
P1A P 0.07244(19) 0.4625(3) 0.3530(2) 0.0295(11) Uani 0.5 1 d . U P A 1
O1 O 0.1111(6) 0.3794(10) 0.3912(8) 0.051(4) Uani 0.5 1 d . U P A 1
P1B P 0.04120(19) 0.5244(4) 0.3352(2) 0.0353(12) Uani 0.5 1 d D U P A 2
O2 O -0.0076(5) 0.5835(12) 0.3024(8) 0.049(4) Uani 0.5 1 d D U P A 2
P2 P 0.10044(8) 0.79828(16) 0.37188(10) 0.0214(5) Uani 1 1 d . . . . .
P3 P 0.07183(9) 0.96368(17) 0.49318(12) 0.0284(5) Uani 1 1 d . . . . .
P4 P 0.10772(9) 0.93530(18) 0.23423(11) 0.0306(6) Uani 1 1 d . . . . .
O3 O 0.1904(2) 0.7064(4) 0.5162(3) 0.0220(12) Uani 1 1 d . U . . .
O4 O 0.1740(2) 0.5520(4) 0.4393(3) 0.0242(13) Uani 1 1 d . . . . .
O5 O 0.1924(2) 0.8811(4) 0.5616(3) 0.0264(13) Uani 1 1 d . . . . .
O6 O 0.2101(2) 0.6962(4) 0.4008(3) 0.0212(12) Uani 1 1 d . . . . .
O7 O 0.0713(2) 0.5305(5) 0.4058(3) 0.0339(16) Uani 1 1 d . . . . .
O8 O 0.2213(2) 0.8861(4) 0.4729(3) 0.0208(12) Uani 1 1 d . . . . .
O9 O 0.1373(2) 0.8368(4) 0.3525(3) 0.0238(13) Uani 1 1 d . . . . .
O10 O 0.1378(2) 1.0204(4) 0.3991(3) 0.0310(15) Uani 1 1 d . . . . .
O11 O 0.0889(3) 0.8669(5) 0.5231(3) 0.0339(15) Uani 1 1 d . . . . .
O12 O 0.1114(2) 0.6934(4) 0.3850(3) 0.0242(13) Uani 1 1 d . . . . .
O13 O 0.2272(2) 0.8660(4) 0.3635(3) 0.0240(13) Uani 1 1 d . . . . .
O14 O 0.0800(2) 0.6909(4) 0.4726(3) 0.0288(14) Uani 1 1 d . . . . .
O15 O 0.1122(3) 0.6846(6) 0.2728(3) 0.046(2) Uani 1 1 d . . . . .
O17 O 0.1432(3) 0.9937(5) 0.2956(3) 0.0410(18) Uani 1 1 d . . . . .
O18 O 0.1519(3) 0.5405(4) 0.5380(3) 0.0321(15) Uani 1 1 d . . . . .
O19 O 0.0429(2) 0.8118(4) 0.3168(3) 0.0251(13) Uani 1 1 d . . . . .
O20 O 0.2374(2) 1.0427(4) 0.4149(3) 0.0311(15) Uani 1 1 d . . . . .
O21 O -0.0590(3) 0.9779(4) 0.4657(4) 0.0374(16) Uani 1 1 d . . . . .
O23 O 0.1369(2) 0.8456(5) 0.2392(3) 0.0361(16) Uani 1 1 d . . . . .
O24 O 0.0827(3) 0.5330(6) 0.3127(4) 0.063(3) Uani 1 1 d . . . . .
O25 O 0.1169(2) 0.8453(4) 0.4360(3) 0.0225(13) Uani 1 1 d . . . . .
O26 O 0.2130(3) 0.7058(5) 0.2869(3) 0.0380(16) Uani 1 1 d . . . . .
O27 O 0.0219(3) 0.9573(5) 0.4234(3) 0.0374(16) Uani 1 1 d . . . . .
O28 O 0.1161(2) 1.0127(4) 0.4923(3) 0.0316(15) Uani 1 1 d . . . . .
O29 O 0.2202(3) 1.0532(5) 0.5324(3) 0.0358(16) Uani 1 1 d . . . . .
O30 O 0.0550(2) 0.9092(5) 0.2243(3) 0.0364(16) Uani 1 1 d . . . . .
O31 O 0.0193(3) 0.4246(6) 0.3100(4) 0.052(2) Uani 1 1 d . . . . .
O32 O 0.1606(3) 0.7315(5) 0.6062(3) 0.0357(16) Uani 1 1 d . . . . .
O33 O 0.1822(4) 0.5278(5) 0.3306(4) 0.057(2) Uani 1 1 d . . . . .
O34 O -0.1003(3) 0.9904(6) 0.3230(3) 0.060(3) Uani 1 1 d . . . . .
N1 N -0.0311(3) 1.1601(5) 0.4018(3) 0.045(2) Uani 1 1 d D U . . .
N2 N -0.0061(5) 1.3110(5) 0.4339(4) 0.084(4) Uani 1 1 d D U . . .
N3 N -0.1790(4) 1.1770(8) 0.2134(5) 0.108(4) Uani 1 1 d D U . . .
H3A H -0.166175 1.122923 0.216746 0.130 Uiso 1 1 calc R U . . .
N4 N -0.2156(4) 1.2995(5) 0.2275(4) 0.114(4) Uani 1 1 d D U . . .
N5 N -0.1429(4) 1.6799(6) 0.3839(5) 0.108(4) Uani 1 1 d D U . . .
N6 N -0.1635(6) 1.7516(7) 0.4474(6) 0.134(5) Uani 1 1 d D U . . .
H6 H -0.171193 1.762651 0.475471 0.161 Uiso 1 1 calc R U . . .
C1 C -0.0064(6) 1.2222(5) 0.4513(5) 0.088(4) Uani 1 1 d D U . . .
H1 H 0.009327 1.204950 0.494511 0.106 Uiso 1 1 calc R U . . .
C2 C -0.0487(7) 1.2141(6) 0.3485(4) 0.114(6) Uani 1 1 d D U . . .
H2 H -0.064815 1.193365 0.305937 0.136 Uiso 1 1 calc R U . . .
C3 C -0.0388(6) 1.3037(7) 0.3680(4) 0.099(5) Uani 1 1 d D U . . .
H3 H -0.052771 1.353698 0.339791 0.119 Uiso 1 1 calc R U . . .
C4 C 0.0225(4) 1.3910(7) 0.4764(7) 0.108(6) Uani 1 1 d D U . . .
H4A H 0.042775 1.420923 0.461991 0.130 Uiso 1 1 calc R U . . .
H4B H 0.047062 1.369838 0.520727 0.130 Uiso 1 1 calc R U . . .
C5 C -0.0160(5) 1.4605(9) 0.4751(8) 0.101(6) Uani 1 1 d D U . . .
H5A H -0.038258 1.429863 0.486372 0.121 Uiso 1 1 calc R U . . .
H5B H -0.038675 1.485965 0.431689 0.121 Uiso 1 1 calc R U . . .
C6 C -0.2060(5) 1.3230(9) 0.1809(5) 0.151(9) Uani 1 1 d D U . . .
H6A H -0.212935 1.379352 0.159736 0.182 Uiso 1 1 calc R U . . .
C7 C -0.1839(6) 1.2462(7) 0.1721(6) 0.104(5) Uani 1 1 d D U . . .
H7 H -0.173792 1.241743 0.142864 0.124 Uiso 1 1 calc R U . . .
C8 C -0.1986(5) 1.2105(6) 0.2482(5) 0.084(3) Uani 1 1 d D U . . .
H8 H -0.200128 1.178826 0.279911 0.101 Uiso 1 1 calc DR U . . .
C9 C -0.2283(4) 1.3855(7) 0.2504(7) 0.140(5) Uani 1 1 d D U . . .
H9A H -0.226273 1.359184 0.287367 0.168 Uiso 1 1 d R U . . .
H9B H -0.262913 1.411784 0.222427 0.168 Uiso 1 1 d R U . . .
C10 C -0.1783(5) 1.4394(8) 0.2995(9) 0.153(5) Uani 1 1 d D U . . .
H10A H -0.160371 1.455754 0.278873 0.184 Uiso 1 1 d DR U . . .
H10B H -0.154231 1.405846 0.338743 0.184 Uiso 1 1 d R U . . .
C11 C -0.1907(5) 1.5355(8) 0.3130(10) 0.148(5) Uani 1 1 d D U . . .
H11A H -0.204037 1.520756 0.339235 0.178 Uiso 1 1 d R U . . .
H11B H -0.218137 1.565045 0.273645 0.178 Uiso 1 1 d DR U . . .
C12 C -0.1394(5) 1.5909(8) 0.3533(8) 0.125(5) Uani 1 1 d D U . . .
H12A H -0.112756 1.551618 0.387943 0.150 Uiso 1 1 calc R U . . .
H12B H -0.127144 1.606302 0.325618 0.150 Uiso 1 1 calc R U . . .
C13 C -0.1273(5) 1.7700(6) 0.3866(6) 0.117(5) Uani 1 1 d D U . . .
H13 H -0.109466 1.795738 0.369556 0.141 Uiso 1 1 calc R U . . .
C14 C -0.1449(5) 1.8118(10) 0.4213(5) 0.131(5) Uani 1 1 d D U . . .
H14 H -0.144336 1.875360 0.426701 0.157 Uiso 1 1 calc R U . . .
C15 C -0.1668(5) 1.6693(8) 0.4174(5) 0.121(5) Uani 1 1 d D U . . .
H15 H -0.182459 1.615582 0.419504 0.145 Uiso 1 1 calc R U . . .
O1W O -0.1880(6) 1.0216(10) 0.3350(7) 0.144(6) Uani 1 1 d D U . . .
H1WA H -0.194834 1.065809 0.352338 0.215 Uiso 1 1 d DR U . . .
H1WB H -0.169514 1.042469 0.321148 0.215 Uiso 1 1 d DR U . . .
O2W O 0.000000 1.2082(17) 0.250000 0.252(17) Uani 1 2 d DS TU P . .
H2WA H -0.018810 1.178870 0.210930 0.378 Uiso 1 1 d DR U . . .
O4W O -0.0341(2) 1.0211(5) 0.1758(3) 0.0383(17) Uani 1 1 d D . . . .
O5W O 0.0161(3) 0.7764(6) 0.1096(5) 0.066(3) Uani 1 1 d . U . . .
O3W O 0.0113(6) 0.6317(12) 0.1886(7) 0.044(4) Uani 0.5 1 d . U P B 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O18 Mo1 O14 105.1(3) . . ?
O18 Mo1 O3 102.4(3) . . ?
O14 Mo1 O3 95.8(3) . . ?
O18 Mo1 O7 95.2(3) . . ?
O14 Mo1 O7 87.5(3) . . ?
O3 Mo1 O7 160.4(2) . . ?
O18 Mo1 O4 98.5(3) . . ?
O14 Mo1 O4 155.2(2) . . ?
O3 Mo1 O4 86.4(2) . . ?
O7 Mo1 O4 82.7(3) . . ?
O18 Mo1 O12 170.8(3) . . ?
O14 Mo1 O12 83.1(2) . . ?
O3 Mo1 O12 80.5(2) . . ?
O7 Mo1 O12 80.8(2) . . ?
O4 Mo1 O12 72.8(2) . . ?
O18 Mo1 Mo3 100.5(2) . . ?
O14 Mo1 Mo3 48.40(19) . . ?
O3 Mo1 Mo3 49.06(17) . . ?
O7 Mo1 Mo3 135.7(2) . . ?
O4 Mo1 Mo3 134.35(17) . . ?
O12 Mo1 Mo3 88.10(16) . . ?
O20 Mo2 O10 104.2(3) . . ?
O20 Mo2 O8 102.9(3) . . ?
O10 Mo2 O8 95.6(3) . . ?
O20 Mo2 O17 98.4(3) . . ?
O10 Mo2 O17 84.8(3) . . ?
O8 Mo2 O17 158.0(2) . . ?
O20 Mo2 O13 94.7(3) . . ?
O10 Mo2 O13 159.8(2) . . ?
O8 Mo2 O13 86.9(2) . . ?
O17 Mo2 O13 85.6(3) . . ?
O20 Mo2 O9 168.0(3) . . ?
O10 Mo2 O9 87.1(2) . . ?
O8 Mo2 O9 79.4(2) . . ?
O17 Mo2 O9 78.6(2) . . ?
O13 Mo2 O9 73.6(2) . . ?
O20 Mo2 Mo4 101.1(2) . . ?
O10 Mo2 Mo4 48.04(19) . . ?
O8 Mo2 Mo4 48.87(17) . . ?
O17 Mo2 Mo4 132.0(2) . . ?
O13 Mo2 Mo4 135.17(16) . . ?
O9 Mo2 Mo4 89.27(15) . . ?
O32 Mo3 O14 104.4(3) . . ?
O32 Mo3 O3 102.3(3) . . ?
O14 Mo3 O3 95.5(2) . . ?
O32 Mo3 O11 97.1(3) . . ?
O14 Mo3 O11 88.8(3) . . ?
O3 Mo3 O11 158.3(3) . . ?
O32 Mo3 O5 96.8(3) . . ?
O14 Mo3 O5 158.1(2) . . ?
O3 Mo3 O5 85.2(2) . . ?
O11 Mo3 O5 83.0(3) . . ?
O32 Mo3 O25 170.2(3) . . ?
O14 Mo3 O25 83.7(2) . . ?
O3 Mo3 O25 82.0(2) . . ?
O11 Mo3 O25 77.3(2) . . ?
O5 Mo3 O25 74.7(2) . . ?
O32 Mo3 Mo1 99.8(2) . . ?
O14 Mo3 Mo1 47.89(18) . . ?
O3 Mo3 Mo1 49.30(17) . . ?
O11 Mo3 Mo1 136.2(2) . . ?
O5 Mo3 Mo1 133.91(17) . . ?
O25 Mo3 Mo1 89.68(15) . . ?
O29 Mo4 O10 104.3(3) . . ?
O29 Mo4 O8 102.3(3) . . ?
O10 Mo4 O8 95.7(3) . . ?
O29 Mo4 O28 97.4(3) . . ?
O10 Mo4 O28 86.6(3) . . ?
O8 Mo4 O28 158.8(2) . . ?
O29 Mo4 O5 98.0(3) . . ?
O10 Mo4 O5 156.6(2) . . ?
O8 Mo4 O5 86.3(2) . . ?
O28 Mo4 O5 83.4(2) . . ?
O29 Mo4 O25 171.2(3) . . ?
O10 Mo4 O25 83.4(2) . . ?
O8 Mo4 O25 80.8(2) . . ?
O28 Mo4 O25 78.6(2) . . ?
O5 Mo4 O25 73.8(2) . . ?
O29 Mo4 Mo2 100.8(2) . . ?
O10 Mo4 Mo2 47.72(19) . . ?
O8 Mo4 Mo2 49.35(15) . . ?
O28 Mo4 Mo2 133.72(18) . . ?
O5 Mo4 Mo2 134.49(17) . . ?
O25 Mo4 Mo2 87.48(14) . . ?
O26 Mo5 O15 105.6(3) . . ?
O26 Mo5 O6 102.6(3) . . ?
O15 Mo5 O6 95.3(3) . . ?
O26 Mo5 O23 96.5(3) . . ?
O15 Mo5 O23 85.9(3) . . ?
O6 Mo5 O23 159.8(3) . . ?
O26 Mo5 O13 98.8(3) . . ?
O15 Mo5 O13 154.5(3) . . ?
O6 Mo5 O13 86.3(2) . . ?
O23 Mo5 O13 84.2(3) . . ?
O26 Mo5 O9 172.1(3) . . ?
O15 Mo5 O9 81.5(3) . . ?
O6 Mo5 O9 79.9(2) . . ?
O23 Mo5 O9 80.3(2) . . ?
O13 Mo5 O9 73.7(2) . . ?
O26 Mo5 Mo6 99.7(2) . . ?
O15 Mo5 Mo6 48.5(2) . . ?
O6 Mo5 Mo6 48.87(16) . . ?
O23 Mo5 Mo6 134.19(19) . . ?
O13 Mo5 Mo6 134.19(16) . . ?
O9 Mo5 Mo6 87.64(15) . . ?
O33 Mo6 O15 105.4(4) . . ?
O33 Mo6 O6 102.0(4) . . ?
O15 Mo6 O6 95.4(3) . . ?
O33 Mo6 O24 95.8(4) . . ?
O15 Mo6 O24 86.2(3) . . ?
O6 Mo6 O24 160.9(3) . . ?
O33 Mo6 O4 98.0(3) . . ?
O15 Mo6 O4 155.7(3) . . ?
O6 Mo6 O4 85.9(2) . . ?
O24 Mo6 O4 84.9(3) . . ?
O33 Mo6 O12 170.2(3) . . ?
O15 Mo6 O12 82.6(3) . . ?
O6 Mo6 O12 82.5(2) . . ?
O24 Mo6 O12 78.9(3) . . ?
O4 Mo6 O12 73.5(2) . . ?
O33 Mo6 Mo5 99.1(3) . . ?
O15 Mo6 Mo5 48.27(19) . . ?
O6 Mo6 Mo5 49.27(16) . . ?
O24 Mo6 Mo5 134.4(2) . . ?
O4 Mo6 Mo5 134.40(17) . . ?
O12 Mo6 Mo5 90.40(15) . . ?
O8 Co1 O8 180.0 7_566 . ?
O8 Co1 O3 84.7(2) 7_566 . ?
O8 Co1 O3 95.3(2) . . ?
O8 Co1 O3 95.3(2) 7_566 7_566 ?
O8 Co1 O3 84.7(2) . 7_566 ?
O3 Co1 O3 180.0 . 7_566 ?
O8 Co1 O6 84.0(2) 7_566 . ?
O8 Co1 O6 96.0(2) . . ?
O3 Co1 O6 96.0(2) . . ?
O3 Co1 O6 84.0(2) 7_566 . ?
O8 Co1 O6 96.0(2) 7_566 7_566 ?
O8 Co1 O6 84.0(2) . 7_566 ?
O3 Co1 O6 84.0(2) . 7_566 ?
O3 Co1 O6 96.0(2) 7_566 7_566 ?
O6 Co1 O6 180.0 . 7_566 ?
O4W Co2 O4W 95.1(4) . 2 ?
O4W Co2 O30 84.0(3) . . ?
O4W Co2 O30 104.5(3) 2 . ?
O4W Co2 O30 104.5(3) . 2 ?
O4W Co2 O30 84.0(3) 2 2 ?
O30 Co2 O30 167.5(4) . 2 ?
O4W Co2 O19 92.5(2) . 2 ?
O4W Co2 O19 167.6(3) 2 2 ?
O30 Co2 O19 86.0(2) . 2 ?
O30 Co2 O19 84.6(2) 2 2 ?
O4W Co2 O19 167.6(3) . . ?
O4W Co2 O19 92.5(2) 2 . ?
O30 Co2 O19 84.6(2) . . ?
O30 Co2 O19 86.0(2) 2 . ?
O19 Co2 O19 81.8(3) 2 . ?
O4W Co2 Co3 137.36(18) . 2 ?
O4W Co2 Co3 109.9(2) 2 2 ?
O30 Co2 Co3 120.0(2) . 2 ?
O30 Co2 Co3 47.7(2) 2 2 ?
O19 Co2 Co3 58.31(17) 2 2 ?
O19 Co2 Co3 47.20(16) . 2 ?
O4W Co2 Co3 109.9(2) . . ?
O4W Co2 Co3 137.36(18) 2 . ?
O30 Co2 Co3 47.7(2) . . ?
O30 Co2 Co3 120.0(2) 2 . ?
O19 Co2 Co3 47.20(15) 2 . ?
O19 Co2 Co3 58.31(17) . . ?
Co3 Co2 Co3 74.28(9) 2 . ?
O3W Co3 O19 94.1(5) . 2 ?
O3W Co3 O30 174.1(5) . . ?
O19 Co3 O30 84.3(2) 2 . ?
O3W Co3 O5W 86.8(5) . . ?
O19 Co3 O5W 94.0(3) 2 . ?
O30 Co3 O5W 87.7(3) . . ?
O3W Co3 O15 77.3(5) . . ?
O19 Co3 O15 155.5(2) 2 . ?
O30 Co3 O15 106.3(3) . . ?
O5W Co3 O15 108.1(3) . . ?
O3W Co3 Co2 135.7(5) . . ?
O19 Co3 Co2 47.42(16) 2 . ?
O30 Co3 Co2 45.56(19) . . ?
O5W Co3 Co2 112.7(2) . . ?
O15 Co3 Co2 127.1(2) . . ?
O21 Co4 O34 102.1(4) . . ?
O21 Co4 O27 108.6(3) . . ?
O34 Co4 O27 107.4(3) . . ?
O21 Co4 N1 121.3(3) . . ?
O34 Co4 N1 105.3(4) . . ?
O27 Co4 N1 111.0(3) . . ?
O31 P1A O24 108.2(5) . . ?
O31 P1A O1 107.5(7) . . ?
O24 P1A O1 122.2(8) . . ?
O31 P1A O7 107.4(5) . . ?
O24 P1A O7 102.2(5) . . ?
O1 P1A O7 108.6(7) . . ?
O7 P1B O2 112.7(8) . . ?
O7 P1B O31 112.2(5) . . ?
O2 P1B O31 103.8(8) . . ?
O7 P1B O24 108.3(5) . . ?
O2 P1B O24 119.2(9) . . ?
O31 P1B O24 99.9(5) . . ?
O19 P2 O25 114.9(3) . . ?
O19 P2 O9 110.2(3) . . ?
O25 P2 O9 106.5(3) . . ?
O19 P2 O12 108.6(3) . . ?
O25 P2 O12 108.2(3) . . ?
O9 P2 O12 108.2(3) . . ?
O28 P3 O21 107.6(4) . 5_576 ?
O28 P3 O11 111.6(4) . . ?
O21 P3 O11 109.1(4) 5_576 . ?
O28 P3 O27 109.7(4) . . ?
O21 P3 O27 108.7(4) 5_576 . ?
O11 P3 O27 110.0(4) . . ?
O30 P4 O34 112.3(4) . 2 ?
O30 P4 O17 113.1(4) . . ?
O34 P4 O17 106.6(4) 2 . ?
O30 P4 O23 108.0(4) . . ?
O34 P4 O23 107.4(5) 2 . ?
O17 P4 O23 109.3(4) . . ?
Mo3 O3 Mo1 81.6(2) . . ?
Mo3 O3 Co1 135.6(3) . . ?
Mo1 O3 Co1 134.7(3) . . ?
Mo6 O4 Mo1 112.9(3) . . ?
Mo4 O5 Mo3 114.4(3) . . ?
Mo6 O6 Mo5 81.9(2) . . ?
Mo6 O6 Co1 134.1(3) . . ?
Mo5 O6 Co1 134.0(3) . . ?
P1B O7 Mo1 135.1(4) . . ?
P1A O7 Mo1 126.6(4) . . ?
Mo4 O8 Mo2 81.8(2) . . ?
Mo4 O8 Co1 136.2(3) . . ?
Mo2 O8 Co1 135.1(3) . . ?
P2 O9 Mo2 128.9(4) . . ?
P2 O9 Mo5 126.3(4) . . ?
Mo2 O9 Mo5 99.9(2) . . ?
Mo2 O10 Mo4 84.2(2) . . ?
P3 O11 Mo3 136.0(4) . . ?
P2 O12 Mo6 124.4(3) . . ?
P2 O12 Mo1 128.1(3) . . ?
Mo6 O12 Mo1 100.2(2) . . ?
Mo5 O13 Mo2 112.0(3) . . ?
Mo1 O14 Mo3 83.7(2) . . ?
Mo5 O15 Mo6 83.3(3) . . ?
Mo5 O15 Co3 118.2(4) . . ?
Mo6 O15 Co3 143.0(4) . . ?
P4 O17 Mo2 132.7(4) . . ?
P2 O19 Co3 138.3(4) . 2 ?
P2 O19 Co2 133.2(4) . . ?
Co3 O19 Co2 85.4(2) 2 . ?
P3 O21 Co4 125.3(4) 5_576 . ?
P4 O23 Mo5 131.1(4) . . ?
P1A O24 Mo6 124.6(5) . . ?
P1B O24 Mo6 132.7(5) . . ?
P2 O25 Mo3 125.1(3) . . ?
P2 O25 Mo4 126.5(3) . . ?
Mo3 O25 Mo4 96.8(2) . . ?
P3 O27 Co4 115.1(4) . . ?
P3 O28 Mo4 134.5(4) . . ?
P4 O30 Co2 149.6(4) . . ?
P4 O30 Co3 116.8(4) . . ?
Co2 O30 Co3 86.7(3) . . ?
P4 O34 Co4 134.9(5) 2 . ?
C1 N1 C2 102.2(8) . . ?
C1 N1 Co4 127.6(6) . . ?
C2 N1 Co4 130.2(7) . . ?
C3 N2 C1 100.0(8) . . ?
C3 N2 C4 131.4(10) . . ?
C1 N2 C4 128.6(9) . . ?
C8 N3 C7 107.5(11) . . ?
C8 N3 H3A 126.3 . . ?
C7 N3 H3A 126.3 . . ?
C8 N4 C6 109.4(10) . . ?
C8 N4 C9 139.2(10) . . ?
C6 N4 C9 109.0(10) . . ?
C13 N5 C15 110.9(10) . . ?
C13 N5 C12 135.0(11) . . ?
C15 N5 C12 114.0(10) . . ?
C15 N6 C14 102.9(13) . . ?
C15 N6 H6 128.6 . . ?
C14 N6 H6 128.6 . . ?
N2 C1 N1 116.2(8) . . ?
N2 C1 H1 121.9 . . ?
N1 C1 H1 121.9 . . ?
C3 C2 N1 108.5(9) . . ?
C3 C2 H2 125.8 . . ?
N1 C2 H2 125.8 . . ?
N2 C3 C2 111.7(9) . . ?
N2 C3 H3 124.2 . . ?
C2 C3 H3 124.2 . . ?
N2 C4 C5 111.2(10) . . ?
N2 C4 H4A 109.4 . . ?
C5 C4 H4A 109.4 . . ?
N2 C4 H4B 109.4 . . ?
C5 C4 H4B 109.4 . . ?
H4A C4 H4B 108.0 . . ?
C4 C5 C5 109.5(11) . 5_586 ?
C4 C5 H5A 109.8 . . ?
C5 C5 H5A 109.8 5_586 . ?
C4 C5 H5B 109.8 . . ?
C5 C5 H5B 109.8 5_586 . ?
H5A C5 H5B 108.2 . . ?
C7 C6 N4 106.3(11) . . ?
C7 C6 H6A 126.8 . . ?
N4 C6 H6A 126.8 . . ?
N3 C7 C6 109.3(12) . . ?
N3 C7 H7 125.3 . . ?
C6 C7 H7 125.3 . . ?
N3 C8 N4 107.5(9) . . ?
N3 C8 H8 126.3 . . ?
N4 C8 H8 126.3 . . ?
N4 C9 C10 112.0(8) . . ?
N4 C9 H9A 97.7 . . ?
C10 C9 H9A 86.5 . . ?
N4 C9 H9B 117.8 . . ?
C10 C9 H9B 125.0 . . ?
H9A C9 H9B 107.9 . . ?
C11 C10 C9 112.5(8) . . ?
C11 C10 H10A 99.9 . . ?
C9 C10 H10A 108.1 . . ?
C11 C10 H10B 112.6 . . ?
C9 C10 H10B 113.8 . . ?
H10A C10 H10B 108.9 . . ?
C10 C11 C12 109.6(8) . . ?
C10 C11 H11A 101.1 . . ?
C12 C11 H11A 109.7 . . ?
C10 C11 H11B 111.5 . . ?
C12 C11 H11B 114.9 . . ?
H11A C11 H11B 109.3 . . ?
N5 C12 C11 116.0(9) . . ?
N5 C12 H12A 108.3 . . ?
C11 C12 H12A 108.3 . . ?
N5 C12 H12B 108.3 . . ?
C11 C12 H12B 108.3 . . ?
H12A C12 H12B 107.4 . . ?
N5 C13 C14 101.9(11) . . ?
N5 C13 H13 129.1 . . ?
C14 C13 H13 129.1 . . ?
C13 C14 N6 114.4(13) . . ?
C13 C14 H14 122.8 . . ?
N6 C14 H14 122.8 . . ?
N6 C15 N5 108.8(11) . . ?
N6 C15 H15 125.6 . . ?
N5 C15 H15 125.6 . . ?
H1WA O1W H1WB 109.1 . . ?
H2WA O2W H2WA 124.1 . 2 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O18 1.674(6) . ?
Mo1 O14 1.931(6) . ?
Mo1 O3 1.982(6) . ?
Mo1 O7 2.084(6) . ?
Mo1 O4 2.102(6) . ?
Mo1 O12 2.283(6) . ?
Mo1 Mo3 2.5868(11) . ?
Mo2 O20 1.673(6) . ?
Mo2 O10 1.928(6) . ?
Mo2 O8 1.987(5) . ?
Mo2 O17 2.048(6) . ?
Mo2 O13 2.112(6) . ?
Mo2 O9 2.264(6) . ?
Mo2 Mo4 2.5924(12) . ?
Mo3 O32 1.682(6) . ?
Mo3 O14 1.946(6) . ?
Mo3 O3 1.975(6) . ?
Mo3 O11 2.040(6) . ?
Mo3 O5 2.097(6) . ?
Mo3 O25 2.328(5) . ?
Mo4 O29 1.675(7) . ?
Mo4 O10 1.937(6) . ?
Mo4 O8 1.973(6) . ?
Mo4 O28 2.037(6) . ?
Mo4 O5 2.089(6) . ?
Mo4 O25 2.375(6) . ?
Mo5 O26 1.687(7) . ?
Mo5 O15 1.945(6) . ?
Mo5 O6 1.981(5) . ?
Mo5 O23 2.046(6) . ?
Mo5 O13 2.084(6) . ?
Mo5 O9 2.281(6) . ?
Mo5 Mo6 2.5877(11) . ?
Mo6 O33 1.677(8) . ?
Mo6 O15 1.951(7) . ?
Mo6 O6 1.969(6) . ?
Mo6 O24 2.081(7) . ?
Mo6 O4 2.085(6) . ?
Mo6 O12 2.264(6) . ?
Co1 O8 2.112(6) 7_566 ?
Co1 O8 2.112(6) . ?
Co1 O3 2.155(6) . ?
Co1 O3 2.155(6) 7_566 ?
Co1 O6 2.186(5) . ?
Co1 O6 2.186(5) 7_566 ?
Co2 O4W 2.066(7) . ?
Co2 O4W 2.066(7) 2 ?
Co2 O30 2.105(7) . ?
Co2 O30 2.105(7) 2 ?
Co2 O19 2.174(6) 2 ?
Co2 O19 2.174(6) . ?
Co2 Co3 2.943(3) 2 ?
Co2 Co3 2.943(3) . ?
Co3 O3W 2.004(17) . ?
Co3 O19 2.167(6) 2 ?
Co3 O30 2.181(7) . ?
Co3 O5W 2.247(11) . ?
Co3 O15 2.283(8) . ?
Co4 O21 1.941(7) . ?
Co4 O34 1.942(7) . ?
Co4 O27 1.966(6) . ?
Co4 N1 1.981(8) . ?
P1A O31 1.459(9) . ?
P1A O24 1.575(9) . ?
P1A O1 1.578(15) . ?
P1A O7 1.652(9) . ?
P1B O7 1.454(8) . ?
P1B O2 1.501(9) . ?
P1B O31 1.571(9) . ?
P1B O24 1.641(10) . ?
P2 O19 1.516(6) . ?
P2 O25 1.531(6) . ?
P2 O9 1.546(6) . ?
P2 O12 1.553(6) . ?
P3 O28 1.532(7) . ?
P3 O21 1.533(7) 5_576 ?
P3 O11 1.537(7) . ?
P3 O27 1.540(7) . ?
P4 O30 1.526(7) . ?
P4 O34 1.528(7) 2 ?
P4 O17 1.537(7) . ?
P4 O23 1.541(8) . ?
N1 C1 1.3600(5) . ?
N1 C2 1.3600(5) . ?
N2 C3 1.3599(5) . ?
N2 C1 1.3600(5) . ?
N2 C4 1.4800(5) . ?
N3 C8 1.3800(5) . ?
N3 C7 1.3800(5) . ?
N3 H3A 0.8600 . ?
N4 C8 1.3800(5) . ?
N4 C6 1.3800(5) . ?
N4 C9 1.5050(4) . ?
N5 C13 1.3800(5) . ?
N5 C15 1.3800(5) . ?
N5 C12 1.5300(5) . ?
N6 C15 1.3800(5) . ?
N6 C14 1.3800(5) . ?
N6 H6 0.8600 . ?
C1 H1 0.9300 . ?
C2 C3 1.3600(5) . ?
C2 H2 0.9300 . ?
C3 H3 0.9300 . ?
C4 C5 1.5300(5) . ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
C5 C5 1.56(3) 5_586 ?
C5 H5A 0.9700 . ?
C5 H5B 0.9700 . ?
C6 C7 1.3800(5) . ?
C6 H6A 0.9300 . ?
C7 H7 0.9300 . ?
C8 H8 0.9300 . ?
C9 C10 1.5300(5) . ?
C9 H9A 0.9600 . ?
C9 H9B 0.9600 . ?
C10 C11 1.5299(5) . ?
C10 H10A 0.9599 . ?
C10 H10B 0.9601 . ?
C11 C12 1.5300(6) . ?
C11 H11A 0.9600 . ?
C11 H11B 0.9600 . ?
C12 H12A 0.9700 . ?
C12 H12B 0.9700 . ?
C13 C14 1.3800(5) . ?
C13 H13 0.9300 . ?
C14 H14 0.9300 . ?
C15 H15 0.9300 . ?
O1W H1WA 0.8596 . ?
O1W H1WB 0.8590 . ?
O2W H2WA 0.9089 . ?
O2W H2WA 0.9088 2 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 P1B O7 Mo1 -90.8(10) . . . . ?
O31 P1B O7 Mo1 152.5(6) . . . . ?
O24 P1B O7 Mo1 43.2(9) . . . . ?
O31 P1A O7 Mo1 -175.2(5) . . . . ?
O24 P1A O7 Mo1 -61.5(6) . . . . ?
O1 P1A O7 Mo1 68.8(8) . . . . ?
O19 P2 O9 Mo2 111.3(4) . . . . ?
O25 P2 O9 Mo2 -13.9(5) . . . . ?
O12 P2 O9 Mo2 -130.0(4) . . . . ?
O19 P2 O9 Mo5 -98.4(4) . . . . ?
O25 P2 O9 Mo5 136.3(4) . . . . ?
O12 P2 O9 Mo5 20.2(5) . . . . ?
O28 P3 O11 Mo3 -28.0(7) . . . . ?
O21 P3 O11 Mo3 -146.8(6) 5_576 . . . ?
O27 P3 O11 Mo3 94.1(6) . . . . ?
O19 P2 O12 Mo6 101.3(4) . . . . ?
O25 P2 O12 Mo6 -133.3(4) . . . . ?
O9 P2 O12 Mo6 -18.3(5) . . . . ?
O19 P2 O12 Mo1 -114.7(4) . . . . ?
O25 P2 O12 Mo1 10.7(5) . . . . ?
O9 P2 O12 Mo1 125.7(4) . . . . ?
O30 P4 O17 Mo2 78.7(7) . . . . ?
O34 P4 O17 Mo2 -157.4(6) 2 . . . ?
O23 P4 O17 Mo2 -41.6(7) . . . . ?
O25 P2 O19 Co3 -73.4(6) . . . 2 ?
O9 P2 O19 Co3 166.3(5) . . . 2 ?
O12 P2 O19 Co3 47.9(6) . . . 2 ?
O25 P2 O19 Co2 78.9(5) . . . . ?
O9 P2 O19 Co2 -41.4(6) . . . . ?
O12 P2 O19 Co2 -159.7(4) . . . . ?
O30 P4 O23 Mo5 -77.1(6) . . . . ?
O34 P4 O23 Mo5 161.6(5) 2 . . . ?
O17 P4 O23 Mo5 46.4(6) . . . . ?
O31 P1A O24 Mo6 -179.4(6) . . . . ?
O1 P1A O24 Mo6 -54.0(11) . . . . ?
O7 P1A O24 Mo6 67.4(7) . . . . ?
O7 P1B O24 Mo6 -33.9(10) . . . . ?
O2 P1B O24 Mo6 96.6(11) . . . . ?
O31 P1B O24 Mo6 -151.4(7) . . . . ?
O19 P2 O25 Mo3 112.1(4) . . . . ?
O9 P2 O25 Mo3 -125.5(4) . . . . ?
O12 P2 O25 Mo3 -9.4(5) . . . . ?
O19 P2 O25 Mo4 -113.4(4) . . . . ?
O9 P2 O25 Mo4 9.0(5) . . . . ?
O12 P2 O25 Mo4 125.1(4) . . . . ?
O28 P3 O27 Co4 -115.6(4) . . . . ?
O21 P3 O27 Co4 1.8(6) 5_576 . . . ?
O11 P3 O27 Co4 121.2(4) . . . . ?
O21 P3 O28 Mo4 148.9(5) 5_576 . . . ?
O11 P3 O28 Mo4 29.2(7) . . . . ?
O27 P3 O28 Mo4 -93.0(6) . . . . ?
O34 P4 O30 Co2 -110.3(9) 2 . . . ?
O17 P4 O30 Co2 10.4(10) . . . . ?
O23 P4 O30 Co2 131.5(8) . . . . ?
O34 P4 O30 Co3 112.3(5) 2 . . . ?
O17 P4 O30 Co3 -127.0(4) . . . . ?
O23 P4 O30 Co3 -5.9(5) . . . . ?
C3 N2 C1 N1 7.7(17) . . . . ?
C4 N2 C1 N1 -172.2(13) . . . . ?
C2 N1 C1 N2 -1.1(14) . . . . ?
Co4 N1 C1 N2 -179.6(9) . . . . ?
C1 N1 C2 C3 -6.2(15) . . . . ?
Co4 N1 C2 C3 172.2(11) . . . . ?
C1 N2 C3 C2 -11.4(19) . . . . ?
C4 N2 C3 C2 168.5(15) . . . . ?
N1 C2 C3 N2 12(2) . . . . ?
C3 N2 C4 C5 69(2) . . . . ?
C1 N2 C4 C5 -111.4(17) . . . . ?
N2 C4 C5 C5 175.4(17) . . . 5_586 ?
C8 N4 C6 C7 1.4(15) . . . . ?
C9 N4 C6 C7 167.5(10) . . . . ?
C8 N3 C7 C6 0.4(15) . . . . ?
N4 C6 C7 N3 -1.1(15) . . . . ?
C7 N3 C8 N4 0.5(14) . . . . ?
C6 N4 C8 N3 -1.2(14) . . . . ?
C9 N4 C8 N3 -160.8(14) . . . . ?
C8 N4 C9 C10 81(2) . . . . ?
C6 N4 C9 C10 -79.2(16) . . . . ?
N4 C9 C10 C11 168.7(15) . . . . ?
C9 C10 C11 C12 -170.8(17) . . . . ?
C13 N5 C12 C11 -131.1(17) . . . . ?
C15 N5 C12 C11 49.6(19) . . . . ?
C10 C11 C12 N5 -166.8(15) . . . . ?
C15 N5 C13 C14 -2.1(14) . . . . ?
C12 N5 C13 C14 178.6(13) . . . . ?
N5 C13 C14 N6 8.5(15) . . . . ?
C15 N6 C14 C13 -11.3(15) . . . . ?
C14 N6 C15 N5 9.2(14) . . . . ?
C13 N5 C15 N6 -4.7(15) . . . . ?
C12 N5 C15 N6 174.8(11) . . . . ?
